J . Phys. Chem. 1989, 93, 6371-6381
Photocatalytic Oxidation of Sulfur Dioxide in Aqueous Suspensions of a-Fe,O, Bruce C. Faust,+Michael R. Hoffmann,* and Detlef W. Bahnemanni W.M . Keck Laboratories, California Institute of Technology, Pasadena, California 91 125 (Received: October 31, 1988; In Final Form: February 3, 1989) The kinetics and mechanism of the photoassisted autoxidation of S(IV) in aqueous colloidal suspensions of a-Fe203have been studied over the pH range of 2-10.5. Similar kinetic behavior toward S(IV) was observed for colloidal suspensions of Ti02. Quantum yields, 4, ranged from 0.08 to 0.3 with a maximum yield found at pH 5.7. Upon band-gap illumination conduction-band electrons and valence-band holes are separated; the trapped electrons are transferred either to surface bound dioxygen or to Fe(II1) sites on or near the surface while the trapped holes accept electrons from adsorbed S(1V) to produce S(V). The formation of S(V) radicals indicates that the reaction proceeds via successive one-electron transfers. The relatively high quantum yields are attributed in part to the desorption of SO3'- from the a-Fe2O3 surface and subsequent initiation of a homogeneous free radical chain autoxidation of S(1V) to S(V1). Kinetic and thermodynamic models for the photoassisted surface chemistry of S(1V) on a-Fe2O3 are presented.
Introduction The catalytic autoxidation of SO2 in deliquescent haze aerosol, clouds, fogs, and hydrometeors appears to be a viable pathway for the rapid formation of sulfuric acid in humid atm~spheres.l-~ Jacob and Hoffmann4 have shown that Fe(II1) and Mn(I1) are the most effective catalysts at ambient concentrations for the autoxidations of S(1V) to S(V1) in cloud and fog water. Although Fe(II1) has been found in high ( N 1 mM) concentrations in atmospheric water droplets, much of this iron is predicted to be in form of solid particles or colloids on the basis of thermodynamic Ferric oxides and oxyhydroxides (a-FezO3, Fe304,a-FeOOH, and y-FeOOH) have been identified as components of airborne particles;13 iron-containing particles such as these are likely to serve as cloud and fog condensation nuclei and to be suspended and/or dissolved in the water droplet that results. Metal oxide semiconductors such as a-Fe203 (hematite) can function either as photosensitizers or as photocatalysts. Absorption of a photon with an energy equal to or greater than the band-gap energy E, of a semiconductor results in the transient formation of an electron/hole pair.
The principal objectives of this paper are to present a detailed study of the kinetics of the heterogeneous photocatalytic oxidation of S(1V) in suspensions of particulate and colloidal a-Fe203 and to present possible mechanisms that take into account the surface chemistry of hematite. Experimental Section Preparation of Fez03 Colloids. The preparation of optically transparent Fez03 colloids was based on the observations made initially by Krecke.21 FeCI3.3H20 crystals (Baker) were ground with a pestle into a fine powder before preparation of aqueous stock solutions in the concentration range of 5-50 mM [Fe3+],,,. Immediately following the preparation of the stock solutions, 300 mL of the FeCl, solution was added dropwise at the rate of 1 drop/s into 1200 mL of boiling water with an initial pH of 7. The solution was subsequently refluxed in a 2-L round-bottom flask. At the end of the reaction, the pH of the solution was found to be within 10% of the value predicted by the following stoichiometry: 2FeC13 3 H 2 0 FezO, 6HCl (1)
(1) Hoffmann, M. R.; Boyce, S . D. Adu. Enuiron. Sci. Technol. 1983, 12, 147-1 89. (2) Hoffmann, M. R.; Jacob, D. J.; In SO2, NO and NO2 Oxidation
In the absence of suitable electron and hole scavengers adsorbed to the surface of a semiconductor particle, recombination occurs within 1 ns. However, when ap ropriate scavengers are present, the valence-band holes, h+vb(E! = 2.3 V (oxidation potential)), function as powerful oxidants while the conduction-band electrons, e-cb (EL = 0.0 V (reduction potential)), function as moderately powerful reductants. Faust,14 Frank and Bard,I5 and Leland and Bard16 have shown that S(IV) (e.g., S02.H20,HSO), or S032-) can be readily oxidized on semiconductor surfaces such as a-Fe203, TiO,, and CdS and also on iron oxide polymorphs such as aFeOOH, P-FeOOH, h-FeOOH, y-FeOOH, and y-FezO3. Hong et al." have previously studied the photocatalytic oxidation of S(IV) by O2 in the presence of TiOz and a hybrid complex of Co(I1) tetrasulfophthalocyanine covalently linked to the surface of TiOz particles. Quantum yields in excess of unity (0.5-300) were observed and attributed to the desorption of SO3'from the Ti02surface and subsequent initiation of a homogeneous free radical chain reaction. In an earlier study, Faust and Hoffmann'* investigated the photoinduced reductive dissolution of a-FezO3 by S(1V) under anoxic conditions over the pH range of 2-4. Likewise, the photoreductive dissolution of y-Fe00H19,32 and a-Fe00H20 by various organic compounds has been investigated. *To whom correspondence should be addressed. ' Forestry & Environmental Studies, Duke University, Durham, N C 27706.
* Institut fur Solarenergieforschung, Sokelantstrasse 5, Hannover, FRG
Mechanisms: Atmospheric Consideration; Calvert, J. G., Ed.; Acid Precipitation Series 3; Butterworth: Boston, 1984; pp 101-172. (3) Penkett, S.A,; Jones, B. M. R.; Brice, K. A,; Eggleton, A. E. J. Afmos. Enuiron. 1979, 13, 123-127. (4) Jacob, D. J.; Hoffmann, M. R. J . Geophys. Res. 1983,88,6611-6621. (5) Waldman, J. M.; Munger, J. W.; Jacob, D. J.; Hoffmann, M. R. Tellus 1985, 378, 91-108. (6) Munger, J. W.; Jacob, D. J.; Waldman, J. W.; Hoffmann, M. R. J . Geophys. Res. 1983, 88, 5109-5121. (7) Jacob, D. J.; Waldman, J. M.; Munger, J. W.; Hoffmann, M. R. Enuiron. Sci. Technol. 1985, 19, 730-735. (8) Waldman, J. M.; Munger, J. W.; Jacob, D. J.; Flagan, R. C.; Morgan, J. J.; Hoffmann, M. R. Science 1982, 218, 677-680. (9) Jacob, D. J.; Waldman, J. M.; Munger, J. W.; Hoffmann, M. R. Tellus 1984, 368, 272-285. (IO) Jacob, D. J.; Waldman, J. M.; Munger, J. W.; Hoffmann, M. R. J . Geophys. Res. 1986, 91, 1089-1096. (11) Jacob, D. J.; Munger, J. W.; Waldman, J. M.; Hoffmann, M. R. J . Geophys. Rev. 1986, 91, 1073-1088. (12) Jacob, D. J.; Shair, F. H.; Waldman, J. M.; Munger, J. W.; Hoffmann, M. R. Atmos. Enuiron. 1987, 21, 1305-1313. (13) Fukasawa, T.; Iwatsuki, M.; Kawabuko, S.;Niyazaki, K. Anal. Chem. 1980, 52, 1784-1787. (14) Faust, B. C. Ph.D. Thesis, California Institute of Technology, Pasadena, CA, 1985. (15) Frank, S . N.; Bard, A. J. J . Phys. Chem. 1977, 81, 1484-1488. (16) Leland, J. K.; Bard, A. J . J . Phys. Chem. 1987, 91, 5076-5083. (17) Hong, A,; Bahnemann, D. W.; Hoffmann, M. R. J . Phys. Chem. 1987, 91, 6245-625 1. (18) Faust, B. C.; Hoffmann, M. R. Enuiron. Sci. Technol. 1986, 20, 943-948. (19) Waite, T. D.; Morel, F. M. M. J . Colloid Interface Sci. 1984, 102, 121-137. (20) Cunningham, K. M.; Goldberg, M. C.; Weiner, E. R. Photochem. Photobiol. 1985, 41, 409-416. (21) Krecke, F. W. 2. Prakt. Cheni. 1871, 3, 286-306.
0 1989 American Chemical Society
Faust et al.
6372 The Journal of Physical Chemistry. Vol. 93, No. 17, I989 1.5
@-aa - Fez03
s o l , 4 8 h 100°C, dialyzed, p H 6 . 2 , 1mM
Figure 1. UV/vis spectra of a-Fe203 transparent colloids and crystals as compared to FeC13 in aqueous solution at 25 OC. (a) I 0 0 pM colloid immediately after preparation at pH 1.9. (b) 100 pM colloid after solvent evaporation and resuspension in water at pH 2.5. (c) 100 pM colloid followed by titration to pH 1 .S, solvent evaporation, and resuspension in water at pH 2.5. For comparison, the UV/vis spectra of a-Fe203 single crystals calculated for a concentration of 100 pM and an aqueous solution of 200 pM FeC13 are also shown.
The resulting clear colloidal suspension was dark red in color and exhibited no detectable light-scattering properties. After initial synthesis, 100-mL aliquots of the Fe203 colloid were dialyzed at 100 OC against water (pHo = 5.6) using a Spectropor/2 28.6mm-diameter dialysis tube (molecular weight cutoff 14000) until M the residual CI-concentration was reduced to a value and the pH of the colloid was 16.0. The optical absorption spectrum of such a colloidal Fez03 preparation is shown in Figure 1 along with the spectrum of the unreacted stock solution (diluted to the appropriated concentration) and the spectrum of a thin film of hematite crystals.22 The onset of absorption of the colloidal preparation starts below 560 nm; this is in excellent agreement with the reported band-gap energy for hematite of 2.2 eV.22 The transparency of the colloidal solution is evident from the absence of an optical absorption above 600 nm. Although the thin-film spectrum of hematite qualitatively resembles the colloidal spectrum, the absorption coefficient of the single-crystal film is considerably larger in the visible region above 380 nm (cf. Figure 1 ). Transmission electron microscopy (TEM) reveals that the colloidal preparation was polydisperse in its size distribution with particle diameters distributed between 3 and 25 nm. While it is very likely that bigger particles exhibit the absorption properties of the bulk material, it has recently been shown that the preparation of extremely small particles (e.g., diameters d
Faust et al.
3 C 0 3
e- 0.0 300
A, Wavelength of lrrodiation (nm) Figure 6. Quantum yield vs wavelength for the photooxidation of 1.O mM S(IV) in a colloidal suspension of 0.1 mM Fe203in the presence of 0.25 mM O2 at pH 6.9.
and competitive adsorption effects become important. Similar kinetic behavior is observed when 0.1 mM K2PtCI6was substituted for 0, as an oxidant, thus preventing the dissolution of the photocatalyst as noted in the experiment described in Figure 3 (dashed line in Figure 4). The initial slope of this curve yielded the same quantum yield as the aerated sample. Depletion of the reactants was reponsible for the apparent slowdown of the sulfite oxidation rate at longer illumination times. Since a marked pH dependence was observed in the experiments described above, the influence of pH on the quantum yield of the S(IV)oxidation over a wider range of conditions was investigated. Figure 5 shows the result of this study (experimental conditions: aerated solutions (0.24 mM 0,) with 1 mM S(IV)and 0.1 mM a-FezO3 colloid): while the quantum yield shows little variation between pH 2 and 5 (the pH range where HS03-dominates S(IV) speciation), there is a marked increase in the observed rate between pH 5 and 6. A further increase in pH, however, results in a considerable decrease of the S(1V)oxidation rate; this occurs at pH values near and above the pH, (7.5) of colloidal Fe,03. Close to the pH,, the colloidal particles will tend to coagulate while above the pH the surface charge will be dominated by negatively charged surface groups (i.e., o-FeO-) and thus will have a much smaller tendency to be adsorbed to the surface due to electrostatic repulsion (as will be shown below in a model of the surface speciation). The wavelength dependence of the quantum yield of the sulfite oxidation measured at pH 6.9 in aerated samples containing 1 mM S(1V)and 0.1 mM Fez03 colloid is shown in Figure 6. N o S(IV)oxidation is observed when illuminations were carried out
/ min Figure 7. Photooxidation of S(IV) on 3.1 X IO-) mol dm-3 colloidal Ti02 at pH 2.0 with A,, = 320 nm in the presence of O2 (-) and Pt4+as electron acceptors (- - -). irradiation lime
with A, > 550 nm (Le., with energies below the band-gap energy of hematite). The increase in quantum yield with an increase in excitation energy could be explained by the presence of smaller particles of hydrous Fe203or hydrous FeOOH that are excited at shorter wavelengths. Of special interest is that the pH, of the colloidal suspension (7.5) is in a range33 more typical of a-FeOOH and y-FeOOH than crystalline a-FezO3 (pH, = 8.5). The photoaction spectrum shown in Figure 6 could therefore be understood in terms of an additive effect of o~yhydroxides~' (e.g., FeOOH. 1.2Hz0 and FeO(3-x),z(OH)x)and crystalline a-Fe2O3 present in the samples. In order to compare the photocatalytic activity of our Fez03 preparations with that of other established photoactive metal oxides, kinetic studies were also performed using colloidal TiOz as a catalyst. Figure 7 shows the oxidation of S(IV)in aqueous solutions containing 3.1 mM TiO, at pH 2 both in the absence and in the presence of oxygen. Under oxic conditions a quantum yield of 0.42 was calculated from the initial slope of the S(IV) depletion (solid line in Figure 7), while a 4 of 0.25 was obtained when Pt4+as PtCIz- acts as the electron acceptor in a Nrsaturated sample (dashed line). The shape of the depletion curves shown in this figure are similar to those obtained for the F q 0 3 photolyses. Adsorption of S(IV) on a-Fe203 in 100-nm Particle Suspensions. Faust and Hoffmann18 have shown that S(IV)is rapidly adsorbed to the surface of a-FezO3. The characteristic time for attainment of equilibrium with respect to the formation of surface complexes in the large particle suspensions is on the order of 1 min. An adsorption isotherm for the surface complexation of S(IV)of the following form was found:
KIXI[S(IV)I~~K,X2[S(IV)laq [s(lv)lads = 1 + K,[S(IV)],,+ 1 + K2[S(1V)laq ( 2 ) where X,and X, are the molar concentrations of the two distinctly are the molar different surface complexes, [S(IV)], and [S(IV)ladS concentrations of all the aqueous and adsorbed S(IV) species, respectively, and K, and K2 are the stability constants for the surface complexes. At pH 2.9 and [a-Fe,O,] = 0.75 mm, K , = 1.1 X IO6 M-I, XI = 1.8 X M, Kz= 2.4 X IO3 M-I, and Xz = 4.4 x 10-5 M. Reaction Stoichiometry. The reaction stoichiometry for the autoxidation of S(1V) was determined to be
The stoichiometry of eq 3 was verified experimentally by deter(31) Mulvaney, P.; Swayambunathan, V.;Grieser, F.; Meisel, D. J . Phys. Chem. 1988, 92, 6132-6140.
Photocatalytic Oxidation of SOz in a-Fez03
The Journal of Physical Chemistry, Vol. 93, No. 17, 1989 6375 I
pH = 2.92 - 2.95
= 0.21 atm. pOZ
A 375 nm x 452 nm
20 Time (min)
Figure 8. Rate of S(IV) photooxidation as a function of [S(IV)] in suspensions of large-particle hematite (Dp N 0.15 pm) with [a-Fe203] = 82.5 pM, pH 2.4, Po2 = 1.0 atm, and X 2 310 nm. Insert gives an expanded scale for the lower left-hand portion of the graph.
mining the analytical concentrations of S(IV), OZ(aq), and Sod2both before and after irradiation of an air-saturated aqueous suspension (pH 2.95) of 100-nm hematite particles ( [a-Fe203] = 82.5 pM) with [S(IV)], = 0.28 mM and [OZl0= 0.24 mM. Results of this experiment gave the following stoichiometric coefficients: A[O,]/A[S(IV)] = 0.41 and A[S(IV)]/A[S(VI)] = -1.01. The discrepancy between experimental and theoretical stoichiometric coefficients (0.41 vs 0.5) is mostly likely due to oxygen leakage into the reactor. Dithionate was observed during the anoxic photooxidation of S(IV) on the small-particle (transparent) suspensions of a-FezO3 (vide supra) but not during the oxidation in the presence of Oz. Even though a-FezO3 and Ozare thermodynamically capable of oxidizing S(IV), O2 is clearly the principal oxidant in this system. In a control experiment, a deoxygenated solution of S(IV) (0.43 mM) and a-Fez03 (0.30 mM; 100 nm particles) under N2 was kept in the dark for 30 min with no detectable production of Fe(I1). However, irradiation with visible light (A = 452 nm) for 3 h produced 12 pM of Fe(II)aq. Experiments with oxygenated suspensions containing S(IV) likewise resulted in the release of small but detectable quantities of Fe(II)aq. In the dark, the rate of dissolution of a 0.75 mM Fe203suspension in the presence of 60 p M S(IV) at pH 2.9 was found to be 0.5 nM min-' ( u = d[Fe(II)]/dt); in the presence of filtered sunlight (A > 300 nm), the rate of release of Fe(I1) to solution was found to increase to 5.3 nM min-'. Although a-Fez03 is thermodynamically capable of oxidizing S(IV), the rate of oxidation S(IV) by hematite is substantially slower than by oxygen (Fe(II1) catalyzed). Kinetics of S ( W ) Oxidation by Ozin Large-Particle (>lo0 nm) Suspensions. As shown in Figure 8, at low [S(IV)] the reaction exhibits an apparent first-order dependence on [S(IV)], while at high [S(IV)] the reaction rate is zero-order with respect to [S(IV)]. Between these concentration extremes the apparent reaction order with respect to [S(IV)] varies between zero and one. This observation is consistent with the concept of saturation kinetics that results from the adsorption of S(IV) on hematite. At lower light intensities, the rate of S(1V) oxidation increases with time (Figure 9). This apparent autocatalytic behavior suggests either the initiation of a free radical chain sequence or a catalytic sequence involving Fe(III)aq generated by oxidation of Fe(II)aq released during photolysis. The rates of S(1V) autoxidation are nearly identical for X = 375 and 452 nm (Figure 9). Similar autocatalytic behavior for S(IV) autoxidation was observed at X = 520 and 600 nm. To check the possibility of a reaction pathway proceeding via the excitation of a surface-bound S(IV) molecule that was not
TIME ( m i n ) Figure 9. Apparent autocatalytic oxidation of S(1V) at two different wavelengths for large-particle suspensions. 10-5
I I l l /
I I l l y
1 I I I I I
PH ~ 2 . 4 4 -2.4%
po,=l.OO otm 10-7
IO-^ [a- Fe,O,]
Figure 10. Apparent zero-order rate constant for S(IV) photooxidation as a function of [a-Fe,O,] (i.e., as a function of total reactive surface area).
dependent on the photochemical properties of a-Fe203, a suspension of alumina, a-A1203(structurally identical with a-FezO3), in the presence of 60 mM S(IV) and 2.5 mM O2 was irradiated at X = 375 nm for 2.5 h. During the illumination period no detectable change in [S(IV)] was observed. The dependence of the observed rate of reaction on the total available surface area is illustrated in Figure 10. The slope of this log-log plot of the pseudo-even-order rate constant, k o w vs [a-FezO,] (e.g., [a-Fe203]a As),is 1, indicating that adsorption to surface active sites is an important pre-equilibrium step in the reaction mechanism. The overall reaction rate measured in terms of the rate of reduction of O2 was also found to be autocatalytic as shown in Figure 1 1. The apparent reaction order with respect to oxygen also exhibited saturation behavior. Discussion The Role of Surface Complexation Formation. The photoassisted heterogeneous solution of S(1V) appears to proceed via rapid formation of Fe(II1)-S(1V) surface complexes formed by ligand exchange with the surface hydroxyl groups. For example, two possible surface complexes are as follows:
The Journal of Physical Chemistry, Vol. 93, No. 17, 1989
Faust et al.
In the first case, a mononuclear monodentate surface complex is formed, while in the second case a monodentate bidentate complexed is formed. In the pH range of 1-3, the overall rate of reaction is limited by [o-FeOSO,-] or [o-FeO,SO] up to the saturation limit imposed by the total number of available surface sites ( - 10 sites/nm2). Enhanced reactivity in the pH range of 5-7 can be attributed either to the more favorable surface complexation of S032-,e.g. kFe/oH \OH2
[01 - Fez 03]= 9 87 x
or to the increased contribution of reaction pathways that occur independently of the surface coordination sites. For example, 0 100 200 SO pH, the particle surfaces iron( 11) porphyrin-dioxygen complexes and Co(I1) Schiff base have a net negative charge due to the increase in the concentration complexes of d i ~ x y g e n . In ~ ~some cases, the 0 2 / 0 2 ' - potential of 0-FeO- and there will be a net electrostatic repulsion of S032can be shifted to (+0.82 V).69 However, in our studies no H 2 0 2 away from the electrical double layer. However, using basic has been detected in aqueous suspensions of hematite particles Gouy-Chapman theory (as shown in Table III), we can calculate under ultra-band-gap excitation in the presence of a variety of the effective concentration of S032-as a function of pH at a electron donors (4 lo's-') is consistent with the conversion of the S:.S-bonded species into the S;.N-bonded species.
Introduction In the past few years, a growing interest in oxidation processes in biological systems has stimulated several investigations of the radiolysis of sulfur-containing amino acids.l-4 It has been shown5 i n the dimeric mixed-valence complex [(R~(NH,!,),( 1.5DTC0)]5+that two neighboring thioether groups facilitate electron transfer in a way that is similar to that in compounds (1) Packer, E. J . J . Chem. SOC.,Perkin Trans. 2 1984, 1015. (2) Buchanan, J. D.; Armstrong, D. A. Int. J . Rodiat. Biol. 1976,30, 115. (3) ill^^, K,-o,; Masloch, B,; Gab], M,; A ~K,-D,~J , A ~~Chem, , ~ sot,, 1981, 103, 2734. (4) Davies, M. J.; Gilbert, B. C.; Norman, R. 0. C. J . Chem. Soc.. Perkin Trans. 2 1983, 73 1. ( 5 ) Stein, C. A.; Taube, H. J . Am. Chem. Soc. 1978, 100, 1635.
where the thioether group is adjacent to another lone-pair donor such as carboxyl or hydroxyl.6 Moreover, interaction of the oxidized sulfur center with the latter groups can result in a lowering Of the reduction potential which, in the case of 2,6-endo,endoand 2,6-exo,endo-thiomethylcarboxylate derivatives of norbornane, et a1.6 was confirmed Similar effects are expected to occur in proteins. They might well evolve from more efficient charge stabilization due to conformational changes leading to favorable mutual positioning of the electron donor-acceptor pairs' A change resulting in a substantial decrease in the reduction potential of (6) Glass, R. S.; Duchek, J. R.; Klug, J. T.; Wilson, G. S. J . Am. Chem. SOC.1977, 99, 7439.
0022-3654/89/2093-6381.$0l.50/00 1989 American Chemical Society